Jul 13, 2013 - School of Chemical Engineering and the Environment, Beijing Institute of ... Mid-Florida Research and Education Center, University of Florida, Apopka, Florida ... effective technologies to remove phosphate from aqueous.
Engineered Biochar Reclaiming Phosphate from Aqueous Solutions: Mechanisms and Potential Application as a Slow-Release Fertilizer Ying Yao,†,‡ Bin Gao,*,† Jianjun Chen,§ and Liuyan Yang⊥ †
Department of Agricultural and Biological Engineering, University of Florida, Gainesville, Florida 32611, United States School of Chemical Engineering and the Environment, Beijing Institute of Technology, Beijing 100081, China § Mid-Florida Research and Education Center, University of Florida, Apopka, Florida 32703, United States ⊥ State Key Laboratory of Pollution Control and Resource Reuse, School of the Environment, Nanjing University, Nanjing 210046, China ‡
S Supporting Information *
ABSTRACT: This work explored the potential application of an engineered biochar prepared from Mg-enriched tomato tissues to reclaim and reuse phosphate (P) from aqueous solution. Findings from batch sorption experiments suggested that, although sorption of P on the biochar was controlled by relatively slow kinetics, the maximum P sorption capacity of the biochar could reach >100 mg·g−1. Mathematical modeling and postsorption characterization results indicated that the sorption was mainly controlled by two mechanisms: precipitation of P through chemical reaction with Mg particles and surface deposition of P on Mg crystals on biochar surfaces. Most of the P retained in the engineered biochar was bioavailable and could be released equally at multiple successive extractions. In addition, the Pladen biochar signiﬁcantly stimulated grass seed germination and growth. These results suggested the postsorption biochar can be cycled back directly to soils as an eﬀective slow-release Pfertilizer.
mentally friendly.13 Most of the traditional engineered carbons (e.g., activated carbon and biochar), however, have limited ability to adsorb P or other anionic nutrients. For example, Namasivayam et al.14 and Bhargava et al.15 reported that the P adsorption capacity of activated carbons derived from coir pith and tamarind nut shell was only about 5.1 mg·g−1 and 5.0 mg·g−1, respectively. Yao et al.16 tested thirteen biochars made from diﬀerent biomass feedstocks and found most of them had little/no ability to sorb phosphate from aqueous solutions. Chen et al.17 reported that magnetic biochars made from irontreated orange peel powders had a P adsorption capacity of only around 1.2 mg·g−1. In order to improve the sorption ability of biochars to aqueous P, several investigations have been conducted to synthesize engineer biochars with novel structures and surface properties.13,17−22 In particular, it has been reported that engineered Mg−biochar nanocomposites with nanosized magnesium oxides (MgO) attached on carbon surfaces within the biochar matrix have superior sorption ability to aqueous P.13,18,20 For example, the MgO−biochar nanocomposites
INTRODUCTION Phosphorus is a limiting nutrient for the growth of organisms and plants and is an indicator of surface water quality.1 Excessive phosphorus from both point and nonpoint sources into natural waters is known to cause eutrophication which is occurring throughout the world.2−5 Dissolved phosphate of ∼0.02 mg·L−1 is considered to have potential that leads to profuse algal growth in waters.6 Accelerated eutrophication not only aﬀects the aquatic ecosystems but also indirectly hinders the economic progress. The combined costs were approximately $2.2 billion annually as a result of eutrophication in U.S. freshwaters.7 It is therefore very important to develop eﬀective technologies to remove phosphate from aqueous solutions prior to their discharge into runoﬀ and natural water bodies. The role of biochar (pyrogenic black carbon derived from incomplete biomass combustion) in political and academic communities has received much attention in recent years. Biochar is widely recognized as an important cost-eﬀective adsorbent storing chemical contaminants including heavy metals, organic compounds, and other environmental pollutions.8−12 The use of carbon/biochar to remove phosphate from aqueous solutions is an emerging and promising concept with plenty of advantages over traditional wastewater treatment technologies, such as lower cost and/or being more environ© 2013 American Chemical Society
Received: Revised: Accepted: Published: 8700
March 24, 2013 July 10, 2013 July 13, 2013 July 13, 2013 dx.doi.org/10.1021/es4012977 | Environ. Sci. Technol. 2013, 47, 8700−8708
Environmental Science & Technology
solutions were prepared by dissolving potassium phosphate monobasic (KH2PO4) in DI water. All the chemicals used in the study are A.C.S certiﬁed and from Fisher Scientiﬁc. P Adsorption. Adsorption kinetics of phosphate on the biochar were examined by mixing 0.1 g of the sorbent with 50 mL of 30.6 mg·L−1 (i.e., 0.3 mM) phosphate solutions in 68 mL digestion vessels (Environmental Express) at room temperature (22 ± 0.5 °C). The vessels were then shaken at 55 rpm in a mechanical shaker. At appropriate time intervals, the vessels were withdrawn and the mixtures were immediately ﬁltered through 0.22 μm pore size nylon membrane ﬁlters (GE cellulose nylon membrane). Adsorption isotherm of phosphate on the biochar was determined similarly by mixing 0.1 g of biochar with 50 mL of phosphate solutions of diﬀerent concentrations ranging from 3.1 to 588.1 mg·L−1 in the digestion vessels. The vessels were shaken in the mechanical shaker for 24 h at room temperature (suﬃcient to reach adsorption equilibrium). The samples were then withdrawn and ﬁltered to determine adsorbed phosphate concentrations. In addition, pH values of solutions before and after phosphate sorption were measured with a pH meter (Fisher Scientiﬁc Accumet Basic AB15). Phosphate concentrations on the solid phase were calculated on the basis of the initial and ﬁnal aqueous concentrations, which were determined by inductively coupled plasma atomic emission spectroscopy (ICP-AES). The postadsorption biochar samples were collected, rinsed with deionized water, and dried at 80 °C for further experiments. Eﬀects of competing compounds on phosphate sorption by the biochar were investigated by adding common coexisting anions (chloride, nitrate, or bicarbonate) or organic matter (humic acid (HA)) to the 30.6 mg·L−1 (0.3 mM/L) phosphate solutions into separate digestion vessels. On the basis of their typical concentrations in wastewater,36−41 50.0 mg·L−1 Cl− (NaCl, 1.4 mM·L−1), 15.0 mg N·L−1 NO3− (NaNO3, 0.24 mM·L−1), 80.0 mg·L−1 HCO3− (NaHCO3, 1.3 mM·L−1), 2.0 mg·L−1 humic acid (HA), or their mixture was used in this work. The ratio of adsorbent to initial P solution was the same as the kinetics/isotherm experiment. The vessels were shaken in the mechanical shaker for 24 h at room temperature. The same procedures were used to determine aqueous and adsorbed phosphate concentrations. All the adsorption experiments were conducted in duplicate, and the average experimental data are reported. Additional measurements were obtained when the duplicates had a diﬀerence larger than 5%. Postsorption Characterization. The physicochemical properties of the engineered biochar have been measured previously and detailed information can be found in Yao et al.19 In this work, the characterization experiments thus were only conducted for the postsorption biochar samples. Scanning electron microscope (SEM) imaging analysis was conducted using a JEOL JSM-6400 scanning microscope. Varying magniﬁcations were used to examine the structure and surface characteristics of the postsorption engineered biochar. Surface element analysis was also conducted simultaneously with the SEM at the same surface locations using energy dispersive X-ray spectroscopy (EDX, Oxford Instruments Link ISIS). The EDX can provide rapid qualitative or, with adequate standards, semiquantitative analysis of elemental composition with a sampling depth of 1−2 μm.42 X-ray diﬀraction (XRD) analysis was carried out to identify any crystallographic structure in the postsorption biochar using a computer-controlled X-ray
synthesized through pyrolyzing anaerobically digested sugar beet tailings 13 or MgCl2-pretreated agricultural residues 20 both showed an extremely high sorption capacity to P (>100 mg·g−1), which is much higher than that of many carbon-based and other commercial adsorbents reported in the literature (